Catastrophic failure of a monolithic zirconia prosthesis Jae-Seung Chang, DDS, PhD,a Woon Ji, DDS,b Chang-Hoon Choi, DDS,c and Sunjai Kim, DDS, PhDd Yong-In Severance Hospital, College of Medicine, Yonsei University, Yong-In, Korea; Gangnam Severance Dental Hospital, College of Dentistry, Yonsei University, Seoul, Korea Recently, monolithic zirconia restorations have received attention as an alternative to zirconia veneered with feldspathic porcelain to eliminate chipping failures of veneer ceramics. In this clinical report, a patient with mandibular edentulism received 4 dental implants in the interforaminal area, and a screw-retained monolithic zirconia prosthesis was fabricated. The patient also received a maxillary complete removable dental prosthesis over 4 anterior roots. At the 18-month follow-up, all of the zirconia cylinders were seen to be fractured, and the contacting abutment surfaces had lost structural integrity. The damaged abutments were replaced with new abutments, and a new prosthesis was delivered with a computer-assisted design and computer-assisted manufacturing fabricated titanium framework with denture teeth and denture base resins. At the 6-month recall, the patient did not have any problems. Dental zirconia has excellent physical properties; however, care should be taken to prevent excessive stresses on the zirconia cylinders when a screw-retained zirconia is planned as a deﬁnitive prosthesis. (J Prosthet Dent 2014;-:---) The introduction of endosteal dental implants has allowed maxillary complete removable dental prostheses (CRDP) to be used with mandibular implantesupported complete ﬁxed dental prostheses (ISCFDP) with patients who are edentulous.1,2 Cast gold alloys are the conventional framework materials for ISCFDPs. Further, computerassisted design and computer-assisted manufacturing (CAD/CAM) technology has enabled the use of titanium alloys and zirconia ceramic as framework materials.3-6 In addition to CAD/ CAM, copy-milling techniques also have been used to fabricate zirconia ceramic frameworks.7,8 Dental zirconia can be veneered with feldspathic porcelain to achieve more esthetic outcomes, although zirconia ceramic prostheses are associated with higher chipping rates than metal ceramic prostheses.9,10 Recently, monolithic
zirconia restorations have been used to eliminate chipping failures, but few clinical studies have shown the outcomes of monolithic zirconia ceramic restorations.7,11 This report describes complications associated with a mandibular monolithic zirconia ceramic, screw-retained ISCFDP.
CLINICAL REPORT A 79-year-old healthy man presented to Department of Prosthodontics, Gangnam Severance Dental Hospital, with concerns chieﬂy of a loose mandibular CRDP and mobility of the maxillary right posterior teeth. The patient had a 1-piece, narrow diameter endosteal dental implant in the mandibular anterior region to retain the CRDP. He reported that 3 implants had been placed in this region approximately 3 years earlier, but 2 implants had been
lost within a year. The patient also had a maxillary partial removable dental prosthesis, but he discontinued its use because of mobility of the abutments (the right second premolar and ﬁrst molar). These teeth were deemed unsalvageable because of advanced periodontal disease. The patient had root rests on both the maxillary central incisors and the left canine. A surveyed crown was placed on the maxillary right canine, which was not mobile or painful (Fig. 1). The patient had no systemic disease that would compromise implant surgery. After a thorough discussion with the patient, a maxillary overdenture on 4 anterior roots and a mandibular, monolithic, zirconia ceramic, screwretained ISCFDP were planned. The possibility of progressive wear of the maxillary denture teeth against the mandibular zirconia ceramic material was a
Supported in part by a faculty research grant, Yonsei University, College of Dentistry for 2013 (6-2013-0078). a
Clinical Assistant Professor, Department of Dentistry, Yong-In Severance Hospital, College of Medicine, Yonsei University. Graduate student, Department of Prosthodontics, Gangnam Severance Dental Hospital, College of Dentistry. c Graduate student, Department of Prosthodontics, Gangnam Severance Dental Hospital, College of Dentistry. d Associate Professor and Chairman, Department of Prosthodontics, Gangnam Severance Dental Hospital, College of Dentistry. b
Chang et al
2 Frontal view of maxillary overdenture and screw-retained monolithic zirconia implantesupported ﬁxed complete denture.
1 Initial panoramic radiograph.
concern, although results of previous studies reported that well-polished zirconia ceramic causes minimal opposing material wear.12,13 Excessive wear of titanium also was expected at the zirconia ceramic cylinderetitanium abutment interface because of the hardness of zirconia ceramic; however, smooth titanium and zirconia ceramic surfaces reportedly do not show different amounts of wear.14 The maxillary right canine was endodontically treated, and its clinical crown was cut to support the planned overdenture. An immediate CRDP was placed after extraction of the maxillary posterior abutments. On the day of implant surgery, the 1piece, mandibular, narrow endosteal dental implant was removed, and 4 internal-connection endosteal dental implants of 4.3-mm diameter and 10-mm length (Inplant; Warantec, Korea) were placed in the interforaminal area; the healing abutments then were placed. The tissue side of the mandibular CRDP was relieved and resurfaced with a resilient, self-polymerizing reline material (Coe-Soft; GC Intl) to avoid premature loading on the healing abutments. After 3 months of healing, 1-piece, titanium deﬁnitive abutments (Multiunit Abutment; Warantec) with ﬂat platforms were placed at the appropriate gingival height. Type III dental stone (CrystalRock; Maruishi Gypsum) was used to fabricate the maxillary, and Type IV dental stone (DieKeen; Heraeus Kulzer) was used for the mandibular deﬁnitive cast.
A veriﬁcation jig was fabricated from the mandibular deﬁnitive cast by connecting the impression copings with an autopolymerizing acrylic resin (Pattern Resin; GC Intl). The 1-screw test was performed in the patient’s mouth to check the ﬁt of the jig and then the jig was cut and rejoined to achieve a passive ﬁt. Both right and left distal abutment analogs were removed from the deﬁnitive cast and repositioned by using the jig, and interim cylinders (Temporary Cylinder; Warantec) were connected to both distal abutment analogs. A ﬁxed resin record base with a wax occlusion rim was fabricated with the interim cylinders to obtain the maxillomandibular relationship record; the denture teeth then were arranged for the maxillary and mandibular prostheses. The cantilever length was set at 1.5 times the anteroposterior spread of the planned endosteal dental implants.15 During the evaluation procedure, the amount of soft tissue support, tooth exposure, and centric relation were reevaluated. The mandibular teeth and gingival contour were impressed by using a high-viscosity silicone elastomeric impression material (Exaﬂex Putty; GC Intl) to form a mold. An autopolymerizing bis-acrylic composite resin (Luxatemp; DMG GmbH) was injected into the mold to fabricate a guide for copy milling a zirconia ceramic block (Prettau; Zirkonzahn GmbH). The milled zirconia framework was characterized with a
The Journal of Prosthetic Dentistry
metal-free brush to simulate tooth and gingival color and sintered in a special furnace (Zirkonofen 600; Zirkonzahn GmbH) to obtain its deﬁnitive mechanical and optical properties. The ﬁt of the prosthesis was checked in the patient’s mouth and considered clinically acceptable, and both the maxillary overdenture and the mandibular ISCFDP were delivered (Fig. 2). A 24-hour follow-up examination was scheduled to identify any soft-tissue irritation or occlusal disharmony. The patient revisited the clinic at 1, 3, 6, 12, and 18 months. At 12 months, he did not report any discomfort or pain. At the 18-month follow-up examination, slight dislodgment of the mandibular prosthesis was noted. When the 4 prosthetic screws were removed, the zirconia ceramic cylinders were found to be fractured (Fig. 3). The interfacial surfaces of the abutments, especially the distal abutments, had severely deteriorated. The 4 abutments were replaced, and an interim ﬁxed dental prosthesis was fabricated from a bis-acrylic composite resin (Luxatemp) by copying the zirconia ceramic prosthesis. The resin guide used for copy milling was converted into a replica by grinding the teeth and gingival portions. A titanium framework was designed and milled on the basis of the replica and the mandibular deﬁnitive cast by using a CAD/CAM system (MyPlant; RaphaBio). The patient returned with repeated fractures of the interim composite resin prosthesis at both the distal
Chang et al
3 Black arrows represent original outline of zirconia cylinder, which lost one-half of integrity because of multiple fractures.
4 Intaglio surface of deﬁnitive prosthesis with computerassisted design and computer-assisted manufacturing fabricated titanium framework with 4 cylinders.
5 A, Frontal view of maxillary overdenture and implant-supported ﬁxed complete denture with denture teeth and denture base resin at 6-month follow-up. Buccal ﬁnish line of titanium framework was apically moved to decrease metal exposure. B, Radiograph with new prosthesis.
cylinder areas in spite of wire reinforcement and the addition of composite resin around the cylinders. Therefore, the length of the distal cantilever was reduced. The ﬁt of the titanium framework was evaluated in the patient’s mouth and the denture teeth were arranged (Fig. 4). The mandibular prosthesis was placed in the patient’s mouth, and the patient resumed the regular follow-up visits (Fig. 5). Scanning electron microscopy was used to analyze the deteriorated abutments (Fig. 6).
DISCUSSION This report presents the unexpected short-term failure of a monolithic,
Chang et al
zirconia ceramic, screw-retained ISCFDP due to fracture of the zirconia ceramic cylinders and structural deterioration of the titanium abutments. The prosthetic failure could have been caused by inaccurate ﬁt between the zirconia ceramic cylinders and the titanium abutments; inadequate cylinder dimensions, which could have accumulated tensile stresses; and excessive cantilever length, which could have produced excessive stress on the zirconia ceramic cylinders. The ISCFDP was fabricated by using a copy-milling technique; therefore, its accuracy depended on operator skill. Thin or irregular structures could have been introduced by the manual grinding
process, and stress accumulation in such areas could have caused the fractures. Bonding or cementing metallic cylinders can compensate for machining errors and provide a passive ﬁt (Fig. 7). The hardness of zirconia ceramic produced excessive wear of the titanium abutments, although a previous study did not show different amounts of wear of smooth titanium and zirconia ceramic surfaces.14 The prosthesis had multiple fractured irregular surfaces with macroroughness at the abutment contact area; therefore, structural deterioration of the titanium abutments was accelerated. Evidence of the continuous hammering of a zirconia
ISCFDPs. However, prosthetic failure was encountered with this treatment. A CAD/CAM-fabricated titanium framework with denture teeth was chosen as the new prosthesis because of its predictable results and long-term clinical success.
6 Scanning electron microscopic image of deteriorated abutment. This abutment lost its entire structural integrity of platforms, and ﬁn-like thin structure was noted at end of platform. Squashed surfaces also had vertical scratch lines, which represent amount of vertical dislodging movement of prosthesis. Hexagon tops represent dent marks that resulted from contact from prosthesis.
Clinicians should be careful when selecting a zirconia ceramic, screwretained prosthesis. The accuracy of the prosthesis, stress accumulation around zirconia ceramic cylinders, and cantilever length should be thoroughly evaluated to prevent failure. An abutment-level prosthesis is a safe option for avoiding damage to the dental implant platform.
7 Metal cylinders. Intaglio surface with metal cylinders in monolithic zirconia prosthesis. Metal cylinders were cemented intraorally with resin cement. ceramic cylinder onto the platform of an abutment is shown in Figure 7. Until now, favorable short-term clinical results of zirconia ceramic, screw-retained frameworks with distal cantilever extensions have been reported.5,7 Both studies used between 5 and 8 implants in an arch to fabricate a zirconia prosthesis. Increased numbers of implants could prevent fracture of zirconia cylinders by reducing the amount of load on each zirconia cylinder. However, more implants also increased the difﬁculty of fabricating a passive ﬁtting prosthesis. In addition, those clinical studies did not describe
the cantilever length. Cantilevers of cast gold alloy screw-retained ISCFDPs should not be longer than 1.5 times the anteroposterior spread of the endosteal dental implants.15 Zirconia ceramic is more vulnerable to tensile stress than gold or titanium alloys; therefore, the maximum cantilever length should be reduced when zirconia ceramic is chosen as the framework material for such prostheses, even though increased numbers of implants could withstand longer cantilever length. Because of its excellent mechanical and biocompatible properties, monolithic zirconia ceramic is an attractive choice for
The Journal of Prosthetic Dentistry
1. Attard NJ, Zarb GA. Long-term treatment outcomes in edentulous patients with implant-ﬁxed prostheses: the Toronto study. Int J Prosthodont 2004;17:417-24. 2. Ekelund JA, Lindquist LW, Carlsson GE, Jemt T. Implant treatment in the edentulous mandible: a prospective study on Brånemark system implants over more than 20 years. Int J Prosthodont 2003;16:602-8. 3. Örtorp A, Jemt T. CNC-milled titanium frameworks supported by implants in the edentulous jaw: a 10-year comparative clinical study. Clin Implant Dent Relat Res 2012;14:88-99. 4. Örtorp A, Jemt T. Clinical experience of CNCmilled titanium frameworks supported by implants in the edentulous jaw: a 3-year interim report. Clin Implant Dent Relat Res 2002;4:104-9. 5. Papaspyridakos P, Lal K. Computer-assisted design/computer-assisted manufacturing zirconia implant ﬁxed complete prostheses: clinical results and technical complications up to 4 years of function. Clin Oral Implants Res 2013;24:659-65. 6. Larsson C, Vult Von Steyern P. Implant-supported full-arch zirconia-based mandibular ﬁxed dental prostheses. Eight-year results from a clinical pilot study. Acta Odontol Scand 2013;71:1118-22. 7. Rojas-Vizcaya F. Full zirconia ﬁxed detachable implant-retained restorations manufactured from monolithic zirconia: clinical report after two years in service. J Prosthodont 2011;20:570-6. 8. Ghazy MH, Madina MM, Aboushelib MN. Inﬂuence of fabrication techniques and artiﬁcial aging on the fracture resistance of different cantilever zirconia ﬁxed dental prostheses. J Adhes Dent 2012; 14:161-6.
Chang et al
9. Raigrodski AJ, Chiche GJ, Potiket N, Hochstedler JL, Mohamed SE, Billiot S, et al. The efﬁcacy of posterior three-unit zirconium-oxide-based ceramic ﬁxed partial dental prostheses: a prospective clinical pilot study. J Prosthet Dent 2006;96:237-44. 10. Raigrodski AJ, Hillstead MB, Meng GK, Chung KH. Survival and complications of zirconia-based ﬁxed dental prostheses: a systematic review. J Prosthet Dent 2012;107: 170-7. 11. Marchack BW, Sato S, Marchack CB, White SN. Complete and partial contour zirconia designs for crowns and ﬁxed dental prostheses: a clinical report. J Prosthet Dent 2011;106:145-52.
Chang et al
5 12. Park JH, Park S, Lee K, Yun KD, Lim HP. Antagonist wear of three CAD/CAM anatomic contour zirconia ceramics. J Prosthet Dent 2014;111:20-9. 13. Ghazal M, Kern M. The inﬂuence of antagonistic surface roughness on the wear of human enamel and nanoﬁlled composite resin artiﬁcial teeth. J Prosthet Dent 2009;101:342-9. 14. Kanbara T, Yajima Y, Yoshinari M. Wear behavior of tetragonal zirconia polycrystal versus titanium and titanium alloy. Biomed Mater 2011;6:021001. 15. McAlarney ME, Stavropoulos DN. Determination of cantilever length-anterior-posterior spread ratio assuming failure criteria to be the compromise of the prosthesis retaining screw-prosthesis joint. Int J Oral Maxillofac Implants 1996;11:331-9.
Corresponding author: Dr Sunjai Kim Eonju-ro 211 Gangnam-gu Seoul 135-270 SOUTH KOREA E-mail: [email protected]
Copyright ª 2014 by the Editorial Council for The Journal of Prosthetic Dentistry.